# Methods of analysis

### 3.4.1 Current density-voltage measurements

The sunlight-to-electricity conversion of a solar cell can be evaluated through the power conversion efficiency (PCE), determined by means of current density-voltage (J-V) measurements. A range of voltages is applied to the solar cell under AM 1.5G illumination conditions. The sunlight radiation is mimicked with a Xenon and a Halogen lamp. The solar cell holder is positioned perpendicularly to these lamps in order to obtain the maximum radiant illumination. A 4-point probe is used to measure the photovoltaic response of the illuminated cell, in order to minimise contact resistance issues. The holder consists of two pins at the cathode of the cell and two pins at the anode, one pin for supplying an input voltage and one for collecting the current. The anode pin is responsible for the voltage ground state. The main parameters of the resulting circuit that can be analysed are:

• Short circuit current Jsc - The generated current when the applied bias is equal to zero.

• Open circuit voltage Voc - The voltage when the input current is equal to the output current, so the net current is zero.

• Maximum power point Pmpp - The point on a current-voltage curve that has the highest I · V product, i.e. the highest power output.

3.4 Methods of analysis 17

• Voltage and current density at the maximum power point Vmpp and Jmpp - The voltage and current density determined at the maximum power point.

• Fill factor FF - The ratio between the product of the Vmppand Jmppand the product of the Voc and the Jsc.

With these parameters, the output power conversion efficiency can simply be calculated through equation 3.1 [40]:

PCE = Pout

Pin = Jsc· Voc·FF

Pin (3.1)

This power conversion efficiency is dependent on the inner resistance of the cell. A solar cell can be analytically modelled as a diode, having a resistance in series and a resistance in parallel (shunt resistance). The electrical circuit that results from this model is visually depicted in figure 3.7.

Figure 3.7: Analytically modelled solar cell as a diode-resistance circuit

For computation of the current density as a function of the net voltage, equation 3.2 applies [41]:

J (V ) = Jph− J0



exp e (V + JRs) nkBT



− 1



− V + J Rs

Rsh (3.2)

Where Jph is the photo-generated current density, J0 is the reverse saturation current density, Rs is the specific series resistance (sheet resistance), kB is the Boltzmann constant, and Rsh is the specific shunt resistance. Shunt resistance indicates the presence of a shunt, which is an alternate path for the current, decreasing the available solar cell voltage. Both series and shunt resistances reduce the fill factor. High values of series resistance will additionally negatively impact the short-circuit current.

The J-V graph is obtained by plotting two curves of the current density J as a function of the applied voltage V. One curve represents the forward scan (increase from 0 V to 1.2 V) and the other the reverse scan (decrease from 1.2 V to 0 V). In perovskite solar cells, the forward and reverse scans do not precisely coincide, which is known as hysteresis.

18 3.4 Methods of analysis

For short integration times, this effect can also cause a deformation in the curve, like an initial “bump” for the reverse scan. This phenomenon can be attributed to a charge accumulation at the interfaces of a perovskite layer, caused by the presence and migration of mobile ions in the material [42, 43]. The algorithm used to determine the PCE during maximum power point tracking is based on a three point weight comparison method [41].

### 3.4.2 Scanning electron microscopy

Scanning electron microscopy (SEM) images the surface of a sample using a beam of electrons accelerated by an applied voltage. Figure 3.8 schematically represents the ray path of such a beam in a SEM setup. These electrons are scattered back by the sample material, and the resulting back-scattered electrons, secondary electrons and X-rays can be detected to image the material. Secondary electrons are emitted after a surface impact by the electron beam, and the removal of inner-shell electrons causes the emission of X-rays.

Back-scattered electrons (BSE) are elastically scattered and they have a higher average energy than secondary electrons (SE), because they originate from deeper inside the material. The electrons are collected by a BSE+SE detector and their energy difference enables the imaging process. The resolution can be scaled down to 1 nm. The specimen has to be smaller than its holder, grounded, and it has to be conductive or covered with a conductive nanometric layer, to avoid charge accumulation. A non-conductive specimen like perovskite is commonly grounded using copper tape to aid the discharge of accumulated charge through the holder. The specimen is inserted for analysis into a vacuum chamber through a loading chamber, to avoid breaking the vacuum of the main chamber. The vacuum enables the correct functioning of the SEM, by avoiding scattering due to the presence of undesired particles in the chamber. The SEM analysis in this thesis was conducted with electrons accelerated by a potential of 5 KeV and a probe current of 7 mA in a JEOL scanning electron microscope.

3.4 Methods of analysis 19

Figure 3.8: Schematised ray path for a scanning electron microscope [44]

### 3.4.3 X-ray diffraction

X-ray diffraction (XRD) is an analysis technique for the crystallography of a material.

This crystalline material acts as a 3D diffraction grating for wavelengths of the size of crystal planes, as satisfied by the X-rays. In the sample holder, the material is subjected to a collimated, monochromatic radiation generated by a cathode ray tube. The diffraction is considered constructive when Bragg’s law, nλ = 2d sin θ, is satisfied, and destructive when it is not [45]. In Bragg’s law, λ refers to the X-ray wavelength, d to the crystal plane spacing, and θ to the angle of incidence of the X-ray. Bragg’s law is illustrated by figure 3.9. The X-rays that are diffracted by the sample are collected by an X-ray detector and categorised. The employed XRD machine for this thesis is an Oxford diffraction machine, Rigaku, and the targets are copper and molybdenum.

20 3.4 Methods of analysis

Figure 3.9: Schematised representation of the functioning of X-ray diffraction through Bragg’s law [45]

### 3.4.4 Transmission electron microscopy

Transmission electron microscopy (TEM) is a method able to provide morphological, crystallographic and chemical analysis. In transmission electron microscopy an electron gun emits electrons, which pass through condenser lenses to tune the illumination aperture and area. Then, a system of lenses enables the imaging procedure by controlling the electron intensity distribution behind the specimen. An electron can be elastically scattered by nuclei with a negligible loss of energy, or diffracted according to Bragg’s law. In the latter case, they can be considered as a Bloch wave field with the lattice periodicity of the specimen, or in-elastically scattered by an interaction with another electron. Two microscopy methods are distinguished: the bright field (BF) or the dark field (DF) imaging.

In the first, the objective aperture selects the transmitted electrons. The contrast is given by crystalline or high mass materials. In dark field imaging, only the scattered electrons are analysed, the transmitted electrons are not considered. The areas with absence of scattered electrons will appear dark. In both methods, electrons are collected by an energy loss spectrometer. X-rays are produced by an interaction of electrons with the specimen. The energy-dispersive X-ray spectroscopy is used in combination with TEM BF and HAADF (high-angle annular dark field imaging) to assess the chemical composition of the samples in relation to their nano-structure. Lamellae from solar cells are prepared for TEM using the focused ion beam (FIB) lift-out method. Since the electrons are to be transmitted through the sample, its thickness can generally not overpass 300 nm.

3.4 Methods of analysis 21

Figure 3.10: Schematised representation of a transmission electron microscope [44]

### 3.4.5 External quantum efficiency

The external quantum efficiency (EQE) is the number of generated electrons in the external circuit by all the incident photons at an established wavelength. The EQE can be measured and graphed by plotting the number of photons that generate electrons against the spectrum of wavelengths for which it is measured, and then normalising it to obtain a probability range. A light beam is generated by a xenon lamp, and split through a grating into radiation waves with different wavelengths. After isolating each wavelength through a monochromator, a chopper is applied to alternately put these in on/off states.

Then, the respective wavelength collimated towards the active area of the solar cell and the produced current is collected and compared to a reference value. The exposed area of the cell to the beam is equal to 1 mm2. During this process, it is important to maintain a constant optical path to avoid inconsistencies. The EQE is finally computed with equation 3.3a, where the spectral response SR is determined by equation 3.3b [46]:

22 3.4 Methods of analysis

EQE = nelectrons nphotons =

JSC

q Ephoto

h·v

=SR · h · c

q · λ (3.3a)

SR = JSC(λ)

EAM1.5g(λ) (3.3b)

The spectral response of the cell under test is compared to that of a reference cell and a monitor cell, in order to keep a baseline and avoid errors. A schematic visualisation of the setup used to determine the EQE is given in figure 3.11. In equational form, the Device Under Test (DUT) spectral response is calculated through equation 3.4:

SRDUT =

stored in calibration file after calibration

z }| {

SRref

| {z }

certified measurement stored in LabView code

· ISC,monitor(λ) ISC,ref(λ)

| {z }

taken during calibration measurement

· ISC,DUT(λ) ISC,monitor(λ)

| {z }

taken during measurement of DUT

(3.4)

At short wavelengths, the EQE is mainly limited by frontal surface recombination, and at long wavelengths it is mainly limited by rear surface recombination. An overall QE reduction is caused by a reflection of the EQE beam on the glass substrate, and parasitic absorption. Furthermore, this reflection limits the diffusion of the beam. Additionally, the EQE measurement is used to determine the short circuit current density of a solar cell.

Figure 3.11: External quantum efficiency measurement scheme [47]

### 3.4.6 Photoluminescence spectroscopy

Photoluminescence spectroscopy is used to contactlessly study the electronic and optical properties of a material. The emission of light is a consequence of the phonon-electron interaction. When photons are absorbed by a material, the resulting light emission is

3.4 Methods of analysis 23

called photoluminescence. After absorbing a photon, an electron is promoted to a higher energy level, resulting in an additional electron in the conduction band and the hole that it leaves in the valence band, with a finite k-moment; an electron-hole recombination is then responsible for the light emission process. The photoluminescent properties of CsPbI2Br is investigated through a fixed-wavelength, diode-pumped solid-state laser (Cobolt Fandango), operating at a wavelength of 514 nm [48]. The laser head collimates and emits a laser beam through a manual shutter. The emitted beam power is long-term stable due to an optical feedback loop. The instrumentation configuration is summed up as follows:

• PL instrumentation: Monovista CRS+ (Spectroscopy and Imaging GmbH)

• Grating groove density: 300 grooves/nm

• Objective: Olympus LC Plan IR objectives for imaging

• Magnification: 50x

• Numerical aperture: 0.65

• Working distance: 4.5mm

• Spectroscopy camera: InGaAs CCD fully integrated camera, cooled at -70 °C The measurements were performed under various illumination power conditions, obtained by attenuating the power of the beam with regard to its spot size and power density. This results in a laser power density of 6 mW/cm2 and a spot size diameter of 50-65 µm, taking into account it has a Gaussian distribution shape.

As the bandgap energy corresponds to the energy of the emitted photons consequential to the passage from valence band to conduction band, it can be determined by inducing that passage and measuring the expelled energy with PL spectroscopy. Furthermore, defects in the material induce defect levels in the bandgap, and can be detected through PL spectroscopy because they exhibit specific radiative transitions. Consequently, two peaks may appear on the resulting PL graph, which implies recombination due to a variety of energy states. Lastly,the evolution of the PL peak positions may provide insights into phase segregation.

### 3.4.7 Absorbance and Absorptance

The Spectro UV-VIS-NIR is employed to indirectly determine the absorbance of a material by measuring its transmittance and reflectance, using the relationship given in equation 3.5. The absorbance is mainly important for determining to what extent a layer absorbs photons in the desired wavelengths, which is necessary for the generation of electricity by the photoactive layer.

24 3.4 Methods of analysis

%Absorbance = 100% − %Reflectance − %Transmittance (3.5) The specific instrument used for this thesis, the Perkin Elmer UV/VIS/NIR lambda 950, consists of the following [49]: Light sources: A halogen gas in the bulb of a tungsten lamp is used to produce a spectrum in the VIS/NIR region (300-3500 nm), and a deuterium gas in the bulb of the tungsten lamp supplies the UV region (175-400 nm). Two monochromators select the same wavelength, to make the cutoff level lower (10−3 · 10−3 = 10−6). Two detectors, one is an Si-based PMT with a spectral response from 150 nm to 900 nm, the other is a cooled InGaAs photodiode with a SR from 800 nm to 2500 nm. An integrating sphere, used to integrate the light distribution of hazy samples in the space.

The absorptance is measured by photothermal deflection spectroscopy (PDS), as this method is able to measure small values of absorptance directly. This technique is based on local heating of a sample under certain sub-gap wavelength light exposure. This light is absorbed and converted into heat by non-radiative recombination, generating a periodic temperature fluctuation that causes periodic changes in the refractive index of the sample.

These changes are then detected from the surrounding environment with a HeNe laser directed parallel to the sample surface. The magnitude of the deflection is finally measured with a position sensitive detector and a lock-in amplifier, through which the absorptance of the sample can be accurately determined. For this thesis, the PDS measurement of the samples is conducted in a basin of Fluorinert, characterised by a large δn/δT .

25